Journal of Nanomaterials

Volumeย 2012ย (2012), Article IDย 953828, 4 pages

http://dx.doi.org/10.1155/2012/953828

## Solubility of Carbon in Nanocrystalline -Iron

Institute of Materials Science, Technische Universitรคt Dresden, 01062 Dresden, Germany

Received 24 February 2012; Accepted 3 May 2012

Academic Editor: Grรฉgoryย Guisbiers

Copyright ยฉ 2012 Alexander Kirchner and Bernd Kieback.

#### Abstract

A thermodynamic model for nanocrystalline interstitial alloys is presented. The equilibrium solid solubility of carbon in -iron is calculated for given grain size. Inside the strained nanograins local variation of the carbon content is predicted. Due to the nonlinear relation between strain and solubility, the averaged solubility in the grain interior increases with decreasing grain size. The majority of the global solubility enhancement is due to grain boundary enrichment however. Therefore the size effect on carbon solubility in nanocrystalline -iron scales with the inverse grain size.

#### 1. Introduction

An enhancement of solid solubility has been found in many bulk nanocrystalline materials, for instance [1, 2]. Often the bigger part of the effect can be attributed to nonequilibrium processing such as mechanical alloying [3]. However quantifying the impact of grain refinement on equilibrium solid solubility is important for understanding the behavior of nanocrystalline alloys upon thermal activation. In this context equilibrium shall be constrained by the assumption of a stable grain size.

The scope of this work is to develop a thermodynamic model of nanocrystalline alloys. It has to comprise both the nanoscale grains and the grain boundary regions, since the fraction of atoms located in those cannot be neglected. The description is based upon the previously published thermodynamic treatment of alloy grain boundaries [4]. There the grain boundaries are approximated by a uniformly dilated lattice retaining the symmetry of the bulk material [5, 6] and are characterized by their volumetric strain .

The interstitial solution of carbon in -iron is chosen as an alloy of practical relevance and experimental accessibility. In pure iron the nanocrystalline state is retained even after prolonged annealing at 650โK [7]. At this temperature and a time of 3600โs, the diffusion length of carbon in bulk iron exceeds 50โ*ฮผ*m [8]. Since the carbon diffusivity will be larger in nanocrystalline iron, this enables chemical equilibration without strong grain growth.

#### 2. Thermodynamic Model of Nanocrystalline Fe-C

The thermodynamic description of a binary Fe-C alloy under volumetric strain is based upon Kaufman and Schlosser's expression [9] for the Helmholtz free energy . The free energy of the strained solid consists of at zero pressure and a second term that accounts for the elastic energy depending on the parameter using the Vinet et al. universal equation of state [10]. The isothermal bulk modulus , the molar volume , and the anharmonicity parameter are given at zero pressure: A two-sublattice model Fe(Va,C) is used to describe the interstitial solution of carbon in -iron. In the second sublattice carbon substitutes normally vacant octahedral sites. Here marks the molar fraction of carbon in the sublattice. Its relation to the carbon content given as the molar fraction is . Conveniently choosing pure -iron and graphite as the reference state, the molar free energy of the unstrained alloy is stated by [11] in units of Joule where is the temperature in Kelvin: Assuming a dilute alloy, and of pure -iron are used in (1). Values of , [12], and [13] at are employed. Their temperature dependence is calculated according to Vinet and coworkers [10] using the coefficient of volumetric thermal expansion [12]. At low solute concentration the molar volume of the alloy varies linearly with , and is obtained. The volume size factor of carbon in -iron is averaged from two publications [14, 15]. The equilibrium between carbon in strained -iron and the reference state graphite is given by .

The strain of the crystallite interior is calculated using Weissmรผller's model [16]. Accordingly local strain in bulk nanocrystalline materials is caused by the fact that the cavities defined by the adjacent grains need to accommodate a finite number of lattice planes. The maximum linear strain is given by the interatomic distance (for iron [12]) and the grain size : The predicted root mean square strain is in good agreement with strain measured in nc-Fe by X-ray diffraction [17, 18]. Here the mean strain is neglected, because with a grain-boundary stress of 1.1โN/m [19] it is more than a magnitude of order smaller than . The volumetric strain is given by the superposition of the linear strain in three dimensions .

Furthermore a thickness of 0.7โnm representing 3-4 monolayers and a value of is used to describe average grain boundaries. This choice of parameters yields a good agreement with an experimental value of the interface free energy of at 1723โK [20].

Finally the resulting global solubility is calculated from the grain boundary and interior compositions with their respective molar fractions as weighting factors: The molar fraction of the atoms located in grain boundaries is corrected for the different atomic densities and converges for and large grain sizes toward .

#### 3. Results and Discussion

Recently *ab initio* methods based on density-functional theory (DFT) allow for highly accurate simulation of carbon solution in -iron. The excess enthalpy of carbon in iron as defined by [21] depending on volumetric strain was calculated at and infinite carbon dilution. The result is presented in Figure 1. Good agreement with the strain dependence of excess enthalpies computed by DFT and a modified embedded-atom method (MEAM) is observed. The calculated derivative of the excess enthalpy with respect to the atomic volume at is as compared to (DFT) and (MEAM).

The maximum linear strain of the grain interior given by (4) can be used to calculate the local volumetric strain assuming three independent axes. For a grain size of 20โnm the linear strain varies locally between and and the volumetric strain between โ0.011 and with the frequency distribution shown in Figure 2. Close to the calculated carbon concentration in equilibrium with graphite at 673โK coincides with the linear theory of thermochemical equilibrium of solids under stress [22]. For large strains nonlinear behavior is observed. At lower values of indicating strong compression, the carbon concentration converges towards zero, which is the physically reasonable behavior.

The expected variation in composition between individual nanograins can be deduced from the range of values calculated for . For a grain size of 20โnm the ratio between the maximum () and the minimum carbon concentration () is 59. This ratio will be even larger for smaller grain sizes. Another notable consequence of the nonlinear trend of is that weighted averaging yields a deviation from bulk solubility despite the strain distribution symmetry. Figure 3 shows the average carbon solubility in the grain interior as a function of inverse grain size. It increases with decreasing grain size slightly. is doubled with respect to the bulk solubility for 11โnm grains.

The carbon concentration in grain boundaries was calculated in equilibrium with graphite assuming it to be independent of curvature and grain size. At a temperature of 673โK the computed value of is *.* This means that carbon is enriched by a factor of in the grain boundaries with respect to the bulk. Atom probe microscopy measurements confirm the presence of a minimum of 2 at.% carbon in -iron grain boundaries [23]. Other experiments at 873โK [24, 25] yielded higher values, expressed as excess densities of carbon at the interface of โ*ฮผ*mol/m^{2}. The corresponding theoretical prediction is lower at โ*ฮผ*mol/m^{2}. The difference may be explained by the strong variation between individual grain boundaries and the information depth of the analytical methods employed. In the case of autoradiography it exceeds the grain boundary thickness of approximately 1โnm by far. The detected amount is likely to include carbon enriched at stress fields around grain boundaries as well. Then the concentration in the grain boundary core is lower than suggests.

Calculating the global solubility according to (5) yields an almost linear relation with the inverse grain size as Figure 3 illustrates. The reason is that the contribution of enriched grain boundaries dominates the size effect. Figure 4 shows the calculated solubility of carbon in nanocrystalline -iron of various grain sizes. Thereafter a pronounced increase in equilibrium carbon solubility is to be expected in nanocrystalline iron in comparison to bulk iron.

#### 4. Conclusions

A thermodynamic model for nanocrystalline -phase Fe-C alloys has been presented. Considering the strained grain interior in equilibrium with graphite local variation of the carbon concentration but only a weak size effect on the average carbon solubility is found. While the extent of enrichment at grain boundaries is not precisely established, grain boundary segregation dominates the solubility increase in the nanocrystalline state. It is concluded that the excess carbon solubility in nanocrystalline iron over bulk iron is proportional to the inverse grain size. At a given temperature the overall solubility follows

#### Acknowledgments

The research of A. Kirchner was supported by Deutsche Forschungsgemeinschaft via the Emmy Noether Programme.

#### References

- H. Gleiter, โNanocrystalline solids,โ
*Journal of Applied Crystallography*, vol. 24, no. 2, pp. 79โ90, 1991. View at Publisher ยท View at Google Scholar ยท View at Scopus - C. D. Terwilliger and Y. M. Chiang, โSize-dependent solute segregation and total solubility in ultrafine polycrystals: Ca in TiO
_{2},โ*Acta Metallurgica Et Materialia*, vol. 43, no. 1, pp. 319โ328, 1995. View at Google Scholar ยท View at Scopus - C. Suryanarayana, โMechanical alloying and milling,โ
*Progress in Materials Science*, vol. 46, no. 1-2, pp. 1โ184, 2001. View at Publisher ยท View at Google Scholar ยท View at Scopus - A. Kirchner and B. Kieback, โThermodynamic model of alloy grain boundaries,โ
*Scripta Materialia*, vol. 64, no. 5, pp. 406โ409, 2011. View at Publisher ยท View at Google Scholar ยท View at Scopus - H. J. Fecht, โIntrinsic instability and entropy stabilization of grain boundaries,โ
*Physical Review Letters*, vol. 65, no. 5, pp. 610โ613, 1990. View at Publisher ยท View at Google Scholar ยท View at Scopus - M. Wagner, โStructure and thermodynamic properties of nanocrystalline metals,โ
*Physical Review B*, vol. 45, no. 2, pp. 635โ639, 1992. View at Publisher ยท View at Google Scholar ยท View at Scopus - T. R. Malow and C. C. Koch, โGrain growth in nanocrystalline iron prepared by mechanical attrition,โ
*Acta Materialia*, vol. 45, no. 5, pp. 2177โ2186, 1997. View at Google Scholar ยท View at Scopus - E. A. Brandes and G. B. Brook, Eds.,
*Smithells Metals Reference Book*, Butterworth Heinemann, Oxford, UK, 1999. - M. Kaufman and H. Schlosser, โA thermodynamic model for pressurized solids,โ
*Journal of Physics*, vol. 7, no. 11, article 03, pp. 2259โ2264, 1995. View at Publisher ยท View at Google Scholar ยท View at Scopus - P. Vinet, J. R. Smith, J. Ferrante, and J. H. Rose, โTemperature effects on the universal equation of state of solids,โ
*Physical Review B*, vol. 35, no. 4, pp. 1945โ1953, 1987. View at Publisher ยท View at Google Scholar ยท View at Scopus - P. Gustafson, โA thermodynamic evaluation of the Fe-C system,โ
*Scandinavian Journal of Metallurgy*, vol. 14, no. 5, pp. 259โ267, 1985. View at Google Scholar ยท View at Scopus - W. Martienssen and H. Warlimont, Eds.,
*Handbook of Condensed Matter and Materials Data*, Springer, Berlin, Germany, 2005. - J. H. Rose, J. R. Smith, F. Guinea, and J. Ferrante, โUniversal features of the equation of state of metals,โ
*Physical Review B*, vol. 29, no. 6, pp. 2963โ2969, 1984. View at Publisher ยท View at Google Scholar ยท View at Scopus - E. J. Fasiska and H. Wagenblast, โDilation of alpha iron by carbon,โ
*Transactions of the Metallurgical Society of AIME*, vol. 239, no. 11, pp. 1818โ1820, 1967. View at Google Scholar - H. W. King, โQuantitative size-factors for interstitial solid solutions,โ
*Journal of Materials Science*, vol. 6, no. 9, pp. 1157โ1167, 1971. View at Publisher ยท View at Google Scholar ยท View at Scopus - J. Weissmüller, โThermodynamics of nanocrystalline solids,โ in
*Nanocrystalline Metals and Oxides*, P. Knauth and J. Schoonman, Eds., Kluwer Academic, New York, NY, USA, 2002. View at Google Scholar - E. Bonetti, L. Del Bianco, L. Pasquini, and E. Sampaolesi, โThermal evolution of ball milled nanocrystalline iron,โ
*Nanostructured Materials*, vol. 12, no. 5, pp. 685โ688, 1999. View at Publisher ยท View at Google Scholar ยท View at Scopus - Y. H. Zhao, H. W. Sheng, and K. Lu, โMicrostructure evolution and thermal properties in nanocrystalline Fe during mechanical attrition,โ
*Acta Materialia*, vol. 49, no. 2, pp. 365โ375, 2001. View at Publisher ยท View at Google Scholar ยท View at Scopus - P. Zimmer and R. Birringer, โMeasuring the interface stress of nanocrystalline iron,โ
*Applied Physics Letters*, vol. 92, no. 8, Article ID 081912, 3 pages, 2008. View at Publisher ยท View at Google Scholar ยท View at Scopus - L. E. Murr,
*Interfacial Phenomena in Metals and Alloys*, Addison-Wesley, New York, NY, USA, 1975. - E. Hristova, R. Janisch, R. Drautz, and A. Hartmaier, โSolubility of carbon in
*α*-iron under volumetric strain and close to the Σ5(310)[001] grain boundary: comparison of DFT and empirical potential methods,โ*Computational Materials Science*, vol. 50, no. 3, pp. 1088โ1096, 2011. View at Publisher ยท View at Google Scholar ยท View at Scopus - F. Larché and J. W. Cahn, โA linear theory of thermochemical equilibrium of solids under stress,โ
*Acta Metallurgica*, vol. 21, no. 8, pp. 1051โ1063, 1973. View at Google Scholar ยท View at Scopus - A. Atrens, J. Q. Wang, K. Stiller, and H. O. Andren, โAtom probe field ion microscope measurements of carbon segregation at an
*α*:*α*grain boundary and service failures by intergranular stress corrosion cracking,โ*Corrosion Science*, vol. 48, no. 1, pp. 79โ92, 2006. View at Publisher ยท View at Google Scholar ยท View at Scopus - J. M. Papazian and D. N. Besherb, โGrain boundary segregation of carbon in iron,โ
*Metallurgical Transactions*, vol. 2, no. 2, pp. 497โ503, 1971. View at Publisher ยท View at Google Scholar ยท View at Scopus - H. Hänsel and H. J. Grabke, โGrain boundary segregation of phosphorus and carbon in ferritic iron,โ
*Scripta Metallurgica*, vol. 20, no. 11, pp. 1641โ1644, 1986. View at Google Scholar ยท View at Scopus